#------------------------------------------------------------------------------
#$Date: 2016-03-23 02:48:26 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179207 $
#$URL: svn://www.crystallography.net/cod/cif/4/31/39/4313906.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4313906
loop_
_publ_author_name
'Aaron P. Holm'
'Seon-Mi Park'
'Cathie L. Condron'
'Marilyn M. Olmstead'
'Hyungrak Kim'
'Peter Klavins'
'Fernande Grandjean'
'Raphaël P. Hermann'
'Gary J. Long'
'Mercouri G. Kanatzidis'
'Susan M. Kauzlarich'
'Sung-Jin Kim'
_publ_section_title
;
 Eu10Mn6Sb13: A New Ternary Rare-Earth Transition-Metal Zintl Phase
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              4660
_journal_page_last               4667
_journal_paper_doi               10.1021/ic034054w
_journal_volume                  42
_journal_year                    2003
_chemical_formula_sum            'Eu10 Mn6 Sb13'
_chemical_formula_weight         3431.99
_chemical_name_common            Eu10Mn6Sb13
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 108.0780(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   15.1791(6)
_cell_length_b                   19.1919(7)
_cell_length_c                   12.2679(4)
_cell_measurement_reflns_used    4924
_cell_measurement_temperature    90(2)
_cell_measurement_theta_max      28.21
_cell_measurement_theta_min      3.49
_cell_volume                     3397.4(2)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Balls & Sticks ver 1.35'
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      90(2)
_diffrn_detector_area_resol_mean 8.3
_diffrn_measured_fraction_theta_full 0.851
_diffrn_measured_fraction_theta_max 0.851
_diffrn_measurement_device_type  'Bruker SMART 1000'
_diffrn_measurement_method       ω
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'normal-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0699
_diffrn_reflns_av_sigmaI/netI    0.0573
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       25
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            17443
_diffrn_reflns_theta_full        28.28
_diffrn_reflns_theta_max         28.28
_diffrn_reflns_theta_min         2.15
_diffrn_standards_decay_%        <0.1
_diffrn_standards_number         '50 frames remeasured'
_exptl_absorpt_coefficient_mu    30.397
_exptl_absorpt_correction_T_max  0.4765
_exptl_absorpt_correction_T_min  0.2055
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'XPREP v. 6.12 (Sheldrick, 2002)'
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    6.710
_exptl_crystal_density_meas      0
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             5772
_exptl_crystal_size_max          0.02
_exptl_crystal_size_mid          0.009
_exptl_crystal_size_min          0.007
_refine_diff_density_max         7.835
_refine_diff_density_min         -3.024
_refine_diff_density_rms         0.534
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.940
_refine_ls_matrix_type           full
_refine_ls_number_parameters     141
_refine_ls_number_reflns         3715
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.940
_refine_ls_R_factor_all          0.0657
_refine_ls_R_factor_gt           0.0410
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0553P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0920
_refine_ls_wR_factor_ref         0.1032
_reflns_number_gt                2603
_reflns_number_total             3715
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic034054wsi20030506_111529.cif
_cod_data_source_block           c2mnew
_cod_original_sg_symbol_H-M      'C 2/m'
_cod_database_code               4313906
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Eu1 Eu 0.0000 0.38126(5) 0.5000 0.00571(19) Uani 1 2 d S . .
Eu2 Eu 0.0000 0.38848(5) 0.0000 0.00654(19) Uani 1 2 d S . .
Eu3 Eu 0.32031(5) 0.38155(3) 0.17082(6) 0.00977(16) Uani 1 1 d . . .
Eu4 Eu 0.23655(5) 0.38185(3) -0.16492(6) 0.00932(16) Uani 1 1 d . . .
Eu5 Eu 0.25214(4) 0.37228(3) 0.49974(5) 0.00638(15) Uani 1 1 d . . .
Eu6 Eu 0.5000 0.34985(5) 0.0000 0.0094(2) Uani 1 2 d S . .
Eu7 Eu 0.5000 0.36425(5) 0.5000 0.0068(2) Uani 1 2 d S . .
Sb1 Sb 0.16615(9) 0.5000 0.63092(11) 0.0063(2) Uani 1 2 d S . .
Sb2 Sb 0.06971(7) 0.38576(4) 0.27610(8) 0.00722(18) Uani 1 1 d . . .
Sb3 Sb 0.16654(8) 0.5000 0.00388(11) 0.0062(2) Uani 1 2 d S . .
Sb4 Sb 0.15425(7) 0.26290(5) 0.00002(8) 0.0093(2) Uani 1 1 d . . .
Sb5 Sb 0.43237(6) 0.34300(5) 0.72569(8) 0.00998(19) Uani 1 1 d . . .
Sb6 Sb 0.35384(9) 0.5000 0.38395(11) 0.0072(2) Uani 1 2 d S . .
Sb7 Sb 0.43265(8) 0.5000 0.73456(10) 0.0039(2) Uiso 1 2 d S . .
Sb8 Sb 0.39915(9) 0.5000 0.00166(11) 0.0088(3) Uani 1 2 d S . .
Sb9 Sb 0.15977(6) 0.25271(4) 0.63756(8) 0.00493(18) Uani 1 1 d . . .
Mn1 Mn 0.1671(2) 0.5000 0.2350(3) 0.0095(6) Uani 1 2 d S . .
Mn2 Mn 0.0503(2) 0.5000 -0.2272(3) 0.0101(6) Uani 1 2 d S . .
Mn3 Mn 0.04289(15) 0.26921(11) 0.77063(19) 0.0099(4) Uani 1 1 d . . .
Mn4 Mn 0.15724(15) 0.26797(11) 0.22855(19) 0.0097(4) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.5866 1.5461 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Eu Eu -0.1578 3.6682 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Sb2 Eu1 Sb2 176.95(4) . 2_556 ?
Sb2 Eu1 Sb1 89.60(3) . . ?
Sb2 Eu1 Sb1 88.35(3) 2_556 . ?
Sb2 Eu1 Sb1 88.35(3) . 5_566 ?
Sb2 Eu1 Sb1 89.60(3) 2_556 5_566 ?
Sb1 Eu1 Sb1 96.09(4) . 5_566 ?
Sb2 Eu1 Sb9 88.27(2) . 2_556 ?
Sb2 Eu1 Sb9 93.89(2) 2_556 2_556 ?
Sb1 Eu1 Sb9 176.39(3) . 2_556 ?
Sb1 Eu1 Sb9 86.76(2) 5_566 2_556 ?
Sb2 Eu1 Sb9 93.89(2) . . ?
Sb2 Eu1 Sb9 88.27(2) 2_556 . ?
Sb1 Eu1 Sb9 86.76(2) . . ?
Sb1 Eu1 Sb9 176.39(3) 5_566 . ?
Sb9 Eu1 Sb9 90.48(3) 2_556 . ?
Sb2 Eu1 Eu5 53.906(19) . . ?
Sb2 Eu1 Eu5 126.264(19) 2_556 . ?
Sb1 Eu1 Eu5 55.76(2) . . ?
Sb1 Eu1 Eu5 128.52(3) 5_566 . ?
Sb9 Eu1 Eu5 120.67(2) 2_556 . ?
Sb9 Eu1 Eu5 55.006(18) . . ?
Sb2 Eu1 Eu5 126.264(19) . 2_556 ?
Sb2 Eu1 Eu5 53.906(19) 2_556 2_556 ?
Sb1 Eu1 Eu5 128.52(3) . 2_556 ?
Sb1 Eu1 Eu5 55.76(2) 5_566 2_556 ?
Sb9 Eu1 Eu5 55.006(18) 2_556 2_556 ?
Sb9 Eu1 Eu5 120.67(2) . 2_556 ?
Eu5 Eu1 Eu5 174.84(3) . 2_556 ?
Sb2 Eu1 Mn3 45.02(4) . 2_556 ?
Sb2 Eu1 Mn3 137.45(4) 2_556 2_556 ?
Sb1 Eu1 Mn3 133.18(4) . 2_556 ?
Sb1 Eu1 Mn3 93.72(4) 5_566 2_556 ?
Sb9 Eu1 Mn3 44.15(4) 2_556 2_556 ?
Sb9 Eu1 Mn3 85.89(4) . 2_556 ?
Eu5 Eu1 Mn3 82.84(3) . 2_556 ?
Eu5 Eu1 Mn3 94.25(3) 2_556 2_556 ?
Sb2 Eu1 Mn3 137.45(4) . . ?
Sb2 Eu1 Mn3 45.02(4) 2_556 . ?
Sb1 Eu1 Mn3 93.72(4) . . ?
Sb1 Eu1 Mn3 133.18(4) 5_566 . ?
Sb9 Eu1 Mn3 85.89(4) 2_556 . ?
Sb9 Eu1 Mn3 44.15(4) . . ?
Eu5 Eu1 Mn3 94.25(3) . . ?
Eu5 Eu1 Mn3 82.84(3) 2_556 . ?
Mn3 Eu1 Mn3 111.84(7) 2_556 . ?
Sb2 Eu2 Sb2 178.14(4) 2 . ?
Sb2 Eu2 Sb3 91.49(3) 2 . ?
Sb2 Eu2 Sb3 89.72(3) . . ?
Sb2 Eu2 Sb3 89.72(3) 2 5_565 ?
Sb2 Eu2 Sb3 91.49(3) . 5_565 ?
Sb3 Eu2 Sb3 99.17(4) . 5_565 ?
Sb2 Eu2 Sb4 89.24(3) 2 2 ?
Sb2 Eu2 Sb4 89.42(3) . 2 ?
Sb3 Eu2 Sb4 174.53(3) . 2 ?
Sb3 Eu2 Sb4 86.25(2) 5_565 2 ?
Sb2 Eu2 Sb4 89.42(3) 2 . ?
Sb2 Eu2 Sb4 89.24(3) . . ?
Sb3 Eu2 Sb4 86.25(2) . . ?
Sb3 Eu2 Sb4 174.53(3) 5_565 . ?
Sb4 Eu2 Sb4 88.34(4) 2 . ?
Sb2 Eu2 Mn2 135.23(5) 2 5_565 ?
Sb2 Eu2 Mn2 46.25(4) . 5_565 ?
Sb3 Eu2 Mn2 87.21(4) . 5_565 ?
Sb3 Eu2 Mn2 46.66(5) 5_565 5_565 ?
Sb4 Eu2 Mn2 96.09(4) 2 5_565 ?
Sb4 Eu2 Mn2 135.01(5) . 5_565 ?
Sb2 Eu2 Mn2 46.25(4) 2 . ?
Sb2 Eu2 Mn2 135.23(5) . . ?
Sb3 Eu2 Mn2 46.66(5) . . ?
Sb3 Eu2 Mn2 87.21(4) 5_565 . ?
Sb4 Eu2 Mn2 135.01(5) 2 . ?
Sb4 Eu2 Mn2 96.09(4) . . ?
Mn2 Eu2 Mn2 110.93(6) 5_565 . ?
Sb2 Eu2 Mn3 45.09(4) 2 1_554 ?
Sb2 Eu2 Mn3 133.36(4) . 1_554 ?
Sb3 Eu2 Mn3 95.39(4) . 1_554 ?
Sb3 Eu2 Mn3 132.82(4) 5_565 1_554 ?
Sb4 Eu2 Mn3 81.30(4) 2 1_554 ?
Sb4 Eu2 Mn3 45.19(4) . 1_554 ?
Mn2 Eu2 Mn3 177.39(5) 5_565 1_554 ?
Mn2 Eu2 Mn3 71.19(4) . 1_554 ?
Sb2 Eu2 Mn3 133.36(4) 2 2_556 ?
Sb2 Eu2 Mn3 45.09(4) . 2_556 ?
Sb3 Eu2 Mn3 132.82(4) . 2_556 ?
Sb3 Eu2 Mn3 95.39(4) 5_565 2_556 ?
Sb4 Eu2 Mn3 45.19(4) 2 2_556 ?
Sb4 Eu2 Mn3 81.30(4) . 2_556 ?
Mn2 Eu2 Mn3 71.19(4) 5_565 2_556 ?
Mn2 Eu2 Mn3 177.39(5) . 2_556 ?
Mn3 Eu2 Mn3 106.74(7) 1_554 2_556 ?
Sb2 Eu2 Mn4 45.21(4) 2 2 ?
Sb2 Eu2 Mn4 133.23(4) . 2 ?
Sb3 Eu2 Mn4 134.47(4) . 2 ?
Sb3 Eu2 Mn4 94.60(4) 5_565 2 ?
Sb4 Eu2 Mn4 45.00(4) 2 2 ?
Sb4 Eu2 Mn4 80.98(4) . 2 ?
Mn2 Eu2 Mn4 131.14(5) 5_565 2 ?
Mn2 Eu2 Mn4 91.42(5) . 2 ?
Mn3 Eu2 Mn4 46.67(5) 1_554 2 ?
Mn3 Eu2 Mn4 88.15(5) 2_556 2 ?
Sb2 Eu2 Mn4 133.23(4) 2 . ?
Sb2 Eu2 Mn4 45.21(4) . . ?
Sb3 Eu2 Mn4 94.60(4) . . ?
Sb3 Eu2 Mn4 134.47(4) 5_565 . ?
Sb4 Eu2 Mn4 80.98(4) 2 . ?
Sb4 Eu2 Mn4 45.00(4) . . ?
Mn2 Eu2 Mn4 91.42(5) 5_565 . ?
Mn2 Eu2 Mn4 131.14(5) . . ?
Mn3 Eu2 Mn4 88.15(5) 1_554 . ?
Mn3 Eu2 Mn4 46.67(5) 2_556 . ?
Mn4 Eu2 Mn4 105.95(7) 2 . ?
Sb6 Eu3 Sb9 90.86(3) . 7_556 ?
Sb6 Eu3 Sb3 85.85(3) . . ?
Sb9 Eu3 Sb3 143.29(3) 7_556 . ?
Sb6 Eu3 Mn3 117.34(5) . 7_556 ?
Sb9 Eu3 Mn3 47.15(4) 7_556 7_556 ?
Sb3 Eu3 Mn3 156.49(5) . 7_556 ?
Sb6 Eu3 Mn1 48.91(5) . . ?
Sb9 Eu3 Mn1 104.81(5) 7_556 . ?
Sb3 Eu3 Mn1 48.07(5) . . ?
Mn3 Eu3 Mn1 151.67(6) 7_556 . ?
Sb6 Eu3 Sb8 91.40(3) . . ?
Sb9 Eu3 Sb8 155.69(3) 7_556 . ?
Sb3 Eu3 Sb8 61.02(3) . . ?
Mn3 Eu3 Sb8 111.41(4) 7_556 . ?
Mn1 Eu3 Sb8 94.81(4) . . ?
Sb6 Eu3 Mn4 101.92(4) . . ?
Sb9 Eu3 Mn4 47.03(4) 7_556 . ?
Sb3 Eu3 Mn4 97.99(4) . . ?
Mn3 Eu3 Mn4 81.77(5) 7_556 . ?
Mn1 Eu3 Mn4 78.49(5) . . ?
Sb8 Eu3 Mn4 154.50(5) . . ?
Sb6 Eu3 Sb4 142.65(3) . . ?
Sb9 Eu3 Sb4 79.56(3) 7_556 . ?
Sb3 Eu3 Sb4 81.17(3) . . ?
Mn3 Eu3 Sb4 81.88(4) 7_556 . ?
Mn1 Eu3 Sb4 98.57(5) . . ?
Sb8 Eu3 Sb4 111.94(3) . . ?
Mn4 Eu3 Sb4 46.39(4) . . ?
Sb6 Eu3 Sb4 163.48(4) . 7 ?
Sb9 Eu3 Sb4 79.44(2) 7_556 7 ?
Sb3 Eu3 Sb4 109.92(3) . 7 ?
Mn3 Eu3 Sb4 46.64(4) 7_556 7 ?
Mn1 Eu3 Sb4 146.57(6) . 7 ?
Sb8 Eu3 Sb4 92.11(3) . 7 ?
Mn4 Eu3 Sb4 81.29(4) . 7 ?
Sb4 Eu3 Sb4 48.90(3) . 7 ?
Sb6 Eu3 Sb5 88.60(3) . 2_656 ?
Sb9 Eu3 Sb5 75.36(3) 7_556 2_656 ?
Sb3 Eu3 Sb5 140.91(3) . 2_656 ?
Mn3 Eu3 Sb5 43.97(4) 7_556 2_656 ?
Mn1 Eu3 Sb5 137.32(5) . 2_656 ?
Sb8 Eu3 Sb5 80.51(3) . 2_656 ?
Mn4 Eu3 Sb5 121.00(4) . 2_656 ?
Sb4 Eu3 Sb5 122.69(3) . 2_656 ?
Sb4 Eu3 Sb5 76.08(3) 7 2_656 ?
Sb6 Eu3 Eu4 137.23(3) . . ?
Sb9 Eu3 Eu4 130.65(3) 7_556 . ?
Sb3 Eu3 Eu4 55.54(2) . . ?
Mn3 Eu3 Eu4 101.26(4) 7_556 . ?
Mn1 Eu3 Eu4 102.33(6) . . ?
Sb8 Eu3 Eu4 55.87(2) . . ?
Mn4 Eu3 Eu4 101.12(4) . . ?
Sb4 Eu3 Eu4 56.07(2) . . ?
Sb4 Eu3 Eu4 56.10(2) 7 . ?
Sb5 Eu3 Eu4 109.25(2) 2_656 . ?
Sb6 Eu3 Eu6 123.24(3) . . ?
Sb9 Eu3 Eu6 108.50(3) 7_556 . ?
Sb3 Eu3 Eu6 103.73(3) . . ?
Mn3 Eu3 Eu6 61.37(4) 7_556 . ?
Mn1 Eu3 Eu6 146.01(4) . . ?
Sb8 Eu3 Eu6 51.24(2) . . ?
Mn4 Eu3 Eu6 130.60(4) . . ?
Sb4 Eu3 Eu6 93.92(2) . . ?
Sb4 Eu3 Eu6 49.71(2) 7 . ?
Sb5 Eu3 Eu6 49.509(17) 2_656 . ?
Eu4 Eu3 Eu6 59.785(15) . . ?
Sb1 Eu4 Sb9 90.08(3) 1_554 1_554 ?
Sb1 Eu4 Sb3 85.21(3) 1_554 . ?
Sb9 Eu4 Sb3 143.39(3) 1_554 . ?
Sb1 Eu4 Mn4 117.26(4) 1_554 7 ?
Sb9 Eu4 Mn4 47.46(4) 1_554 7 ?
Sb3 Eu4 Mn4 157.17(5) . 7 ?
Sb1 Eu4 Sb8 90.09(3) 1_554 . ?
Sb9 Eu4 Sb8 155.31(3) 1_554 . ?
Sb3 Eu4 Sb8 61.15(3) . . ?
Mn4 Eu4 Sb8 111.82(4) 7 . ?
Sb1 Eu4 Mn2 48.95(5) 1_554 . ?
Sb9 Eu4 Mn2 103.88(5) 1_554 . ?
Sb3 Eu4 Mn2 48.00(5) . . ?
Mn4 Eu4 Mn2 151.11(6) 7 . ?
Sb8 Eu4 Mn2 94.74(4) . . ?
Sb1 Eu4 Sb4 142.30(3) 1_554 . ?
Sb9 Eu4 Sb4 80.41(3) 1_554 . ?
Sb3 Eu4 Sb4 81.45(2) . . ?
Mn4 Eu4 Sb4 82.29(4) 7 . ?
Sb8 Eu4 Sb4 113.27(3) . . ?
Mn2 Eu4 Sb4 97.93(5) . . ?
Sb1 Eu4 Sb4 163.49(3) 1_554 7 ?
Sb9 Eu4 Sb4 80.30(2) 1_554 7 ?
Sb3 Eu4 Sb4 110.49(3) . 7 ?
Mn4 Eu4 Sb4 46.77(4) 7 7 ?
Sb8 Eu4 Sb4 93.12(3) . 7 ?
Mn2 Eu4 Sb4 146.51(5) . 7 ?
Sb4 Eu4 Sb4 49.38(3) . 7 ?
Sb1 Eu4 Mn3 101.50(5) 1_554 1_554 ?
Sb9 Eu4 Mn3 47.10(4) 1_554 1_554 ?
Sb3 Eu4 Mn3 98.42(4) . 1_554 ?
Mn4 Eu4 Mn3 81.74(5) 7 1_554 ?
Sb8 Eu4 Mn3 155.85(5) . 1_554 ?
Mn2 Eu4 Mn3 77.83(5) . 1_554 ?
Sb4 Eu4 Mn3 46.72(4) . 1_554 ?
Sb4 Eu4 Mn3 81.78(4) 7 1_554 ?
Sb1 Eu4 Sb5 88.31(3) 1_554 1_554 ?
Sb9 Eu4 Sb5 74.42(2) 1_554 1_554 ?
Sb3 Eu4 Sb5 141.43(3) . 1_554 ?
Mn4 Eu4 Sb5 43.59(4) 7 1_554 ?
Sb8 Eu4 Sb5 80.91(3) . 1_554 ?
Mn2 Eu4 Sb5 137.19(5) . 1_554 ?
Sb4 Eu4 Sb5 123.06(3) . 1_554 ?
Sb4 Eu4 Sb5 76.23(2) 7 1_554 ?
Mn3 Eu4 Sb5 120.12(4) 1_554 1_554 ?
Sb1 Eu4 Eu3 136.24(3) 1_554 . ?
Sb9 Eu4 Eu3 132.41(3) 1_554 . ?
Sb3 Eu4 Eu3 55.25(2) . . ?
Mn4 Eu4 Eu3 102.22(4) 7 . ?
Sb8 Eu4 Eu3 56.46(2) . . ?
Mn2 Eu4 Eu3 101.89(5) . . ?
Sb4 Eu4 Eu3 56.81(2) . . ?
Sb4 Eu4 Eu3 56.97(2) 7 . ?
Mn3 Eu4 Eu3 102.15(4) 1_554 . ?
Sb5 Eu4 Eu3 110.26(3) 1_554 . ?
Sb1 Eu4 Eu6 122.42(3) 1_554 . ?
Sb9 Eu4 Eu6 108.74(3) 1_554 . ?
Sb3 Eu4 Eu6 104.31(3) . . ?
Mn4 Eu4 Eu6 61.38(4) 7 . ?
Sb8 Eu4 Eu6 51.74(2) . . ?
Mn2 Eu4 Eu6 146.44(4) . . ?
Sb4 Eu4 Eu6 95.08(2) . . ?
Sb4 Eu4 Eu6 50.24(2) 7 . ?
Mn3 Eu4 Eu6 131.48(4) 1_554 . ?
Sb5 Eu4 Eu6 49.533(17) 1_554 . ?
Eu3 Eu4 Eu6 60.776(15) . . ?
Sb2 Eu5 Sb5 174.64(3) . . ?
Sb2 Eu5 Sb9 95.67(3) . . ?
Sb5 Eu5 Sb9 80.14(3) . . ?
Sb2 Eu5 Sb1 89.46(3) . . ?
Sb5 Eu5 Sb1 93.75(3) . . ?
Sb9 Eu5 Sb1 88.46(2) . . ?
Sb2 Eu5 Sb6 88.20(3) . . ?
Sb5 Eu5 Sb6 96.19(3) . . ?
Sb9 Eu5 Sb6 174.89(3) . . ?
Sb1 Eu5 Sb6 88.23(3) . . ?
Sb2 Eu5 Sb9 90.05(3) . 7_556 ?
Sb5 Eu5 Sb9 86.86(3) . 7_556 ?
Sb9 Eu5 Sb9 93.20(2) . 7_556 ?
Sb1 Eu5 Sb9 178.30(3) . 7_556 ?
Sb6 Eu5 Sb9 90.13(3) . 7_556 ?
Sb2 Eu5 Eu7 126.43(2) . . ?
Sb5 Eu5 Eu7 54.653(18) . . ?
Sb9 Eu5 Eu7 122.56(3) . . ?
Sb1 Eu5 Eu7 123.94(3) . . ?
Sb6 Eu5 Eu7 56.74(2) . . ?
Sb9 Eu5 Eu7 55.27(2) 7_556 . ?
Sb2 Eu5 Mn4 45.87(4) . . ?
Sb5 Eu5 Mn4 130.17(4) . . ?
Sb9 Eu5 Mn4 88.67(4) . . ?
Sb1 Eu5 Mn4 134.62(4) . . ?
Sb6 Eu5 Mn4 96.43(4) . . ?
Sb9 Eu5 Mn4 45.18(4) 7_556 . ?
Eu7 Eu5 Mn4 95.00(4) . . ?
Sb2 Eu5 Eu1 53.642(18) . . ?
Sb5 Eu5 Eu1 125.30(2) . . ?
Sb9 Eu5 Eu1 57.58(2) . . ?
Sb1 Eu5 Eu1 55.81(2) . . ?
Sb6 Eu5 Eu1 123.09(3) . . ?
Sb9 Eu5 Eu1 124.97(3) 7_556 . ?
Eu7 Eu5 Eu1 179.75(3) . . ?
Mn4 Eu5 Eu1 85.20(4) . . ?
Sb2 Eu5 Eu4 122.14(3) . 1_556 ?
Sb5 Eu5 Eu4 57.70(2) . 1_556 ?
Sb9 Eu5 Eu4 52.036(19) . 1_556 ?
Sb1 Eu5 Eu4 50.14(2) . 1_556 ?
Sb6 Eu5 Eu4 122.96(3) . 1_556 ?
Sb9 Eu5 Eu4 131.35(2) 7_556 1_556 ?
Eu7 Eu5 Eu4 111.177(19) . 1_556 ?
Mn4 Eu5 Eu4 140.07(4) . 1_556 ?
Eu1 Eu5 Eu4 68.726(14) . 1_556 ?
Sb2 Eu5 Eu3 67.02(2) . . ?
Sb5 Eu5 Eu3 113.79(2) . . ?
Sb9 Eu5 Eu3 136.26(2) . . ?
Sb1 Eu5 Eu3 128.89(2) . . ?
Sb6 Eu5 Eu3 48.53(2) . . ?
Sb9 Eu5 Eu3 49.462(18) 7_556 . ?
Eu7 Eu5 Eu3 59.407(13) . . ?
Mn4 Eu5 Eu3 49.89(3) . . ?
Eu1 Eu5 Eu3 120.666(18) . . ?
Eu4 Eu5 Eu3 169.23(2) 1_556 . ?
Sb4 Eu6 Sb4 94.51(4) 7 8 ?
Sb4 Eu6 Sb5 88.63(3) 7 1_554 ?
Sb4 Eu6 Sb5 88.17(3) 8 1_554 ?
Sb4 Eu6 Sb5 88.17(3) 7 2_656 ?
Sb4 Eu6 Sb5 88.63(3) 8 2_656 ?
Sb5 Eu6 Sb5 175.29(5) 1_554 2_656 ?
Sb4 Eu6 Sb8 160.82(3) 7 5_665 ?
Sb4 Eu6 Sb8 104.67(3) 8 5_665 ?
Sb5 Eu6 Sb8 91.59(3) 1_554 5_665 ?
Sb5 Eu6 Sb8 92.57(3) 2_656 5_665 ?
Sb4 Eu6 Sb8 104.67(3) 7 . ?
Sb4 Eu6 Sb8 160.82(3) 8 . ?
Sb5 Eu6 Sb8 92.57(3) 1_554 . ?
Sb5 Eu6 Sb8 91.59(3) 2_656 . ?
Sb8 Eu6 Sb8 56.16(4) 5_665 . ?
Sb4 Eu6 Mn4 45.96(4) 7 7 ?
Sb4 Eu6 Mn4 83.66(4) 8 7 ?
Sb5 Eu6 Mn4 43.85(4) 1_554 7 ?
Sb5 Eu6 Mn4 132.25(4) 2_656 7 ?
Sb8 Eu6 Mn4 134.98(4) 5_665 7 ?
Sb8 Eu6 Mn4 109.90(4) . 7 ?
Sb4 Eu6 Mn4 83.66(4) 7 8 ?
Sb4 Eu6 Mn4 45.96(4) 8 8 ?
Sb5 Eu6 Mn4 132.25(4) 1_554 8 ?
Sb5 Eu6 Mn4 43.85(4) 2_656 8 ?
Sb8 Eu6 Mn4 109.90(4) 5_665 8 ?
Sb8 Eu6 Mn4 134.98(4) . 8 ?
Mn4 Eu6 Mn4 107.19(7) 7 8 ?
Sb4 Eu6 Mn3 83.53(4) 7 8_554 ?
Sb4 Eu6 Mn3 45.86(4) 8 8_554 ?
Sb5 Eu6 Mn3 43.63(4) 1_554 8_554 ?
Sb5 Eu6 Mn3 132.44(4) 2_656 8_554 ?
Sb8 Eu6 Mn3 109.55(4) 5_665 8_554 ?
Sb8 Eu6 Mn3 135.81(4) . 8_554 ?
Mn4 Eu6 Mn3 46.88(5) 7 8_554 ?
Mn4 Eu6 Mn3 88.63(5) 8 8_554 ?
Sb4 Eu6 Mn3 45.86(4) 7 7_556 ?
Sb4 Eu6 Mn3 83.53(4) 8 7_556 ?
Sb5 Eu6 Mn3 132.44(4) 1_554 7_556 ?
Sb5 Eu6 Mn3 43.63(4) 2_656 7_556 ?
Sb8 Eu6 Mn3 135.81(4) 5_665 7_556 ?
Sb8 Eu6 Mn3 109.55(4) . 7_556 ?
Mn4 Eu6 Mn3 88.63(5) 7 7_556 ?
Mn4 Eu6 Mn3 46.88(5) 8 7_556 ?
Mn3 Eu6 Mn3 106.84(7) 8_554 7_556 ?
Sb4 Eu6 Eu4 137.40(3) 7 2_655 ?
Sb4 Eu6 Eu4 58.40(2) 8 2_655 ?
Sb5 Eu6 Eu4 119.388(19) 1_554 2_655 ?
Sb5 Eu6 Eu4 61.453(19) 2_656 2_655 ?
Sb8 Eu6 Eu4 57.40(2) 5_665 2_655 ?
Sb8 Eu6 Eu4 105.25(3) . 2_655 ?
Mn4 Eu6 Eu4 140.95(4) 7 2_655 ?
Mn4 Eu6 Eu4 53.76(3) 8 2_655 ?
Mn3 Eu6 Eu4 95.37(3) 8_554 2_655 ?
Mn3 Eu6 Eu4 95.32(3) 7_556 2_655 ?
Sb4 Eu6 Eu4 58.40(2) 7 . ?
Sb4 Eu6 Eu4 137.40(3) 8 . ?
Sb5 Eu6 Eu4 61.453(19) 1_554 . ?
Sb5 Eu6 Eu4 119.388(19) 2_656 . ?
Sb8 Eu6 Eu4 105.25(3) 5_665 . ?
Sb8 Eu6 Eu4 57.40(2) . . ?
Mn4 Eu6 Eu4 53.76(3) 7 . ?
Mn4 Eu6 Eu4 140.96(4) 8 . ?
Mn3 Eu6 Eu4 95.32(3) 8_554 . ?
Mn3 Eu6 Eu4 95.37(3) 7_556 . ?
Eu4 Eu6 Eu4 162.02(3) 2_655 . ?
Sb5 Eu7 Sb5 165.64(5) 2_656 . ?
Sb5 Eu7 Sb9 81.84(2) 2_656 7_556 ?
Sb5 Eu7 Sb9 88.54(3) . 7_556 ?
Sb5 Eu7 Sb9 88.54(3) 2_656 8 ?
Sb5 Eu7 Sb9 81.84(2) . 8 ?
Sb9 Eu7 Sb9 95.89(4) 7_556 8 ?
Sb5 Eu7 Sb6 96.53(3) 2_656 5_666 ?
Sb5 Eu7 Sb6 94.36(3) . 5_666 ?
Sb9 Eu7 Sb6 172.40(3) 7_556 5_666 ?
Sb9 Eu7 Sb6 91.48(2) 8 5_666 ?
Sb5 Eu7 Sb6 94.36(3) 2_656 . ?
Sb5 Eu7 Sb6 96.53(3) . . ?
Sb9 Eu7 Sb6 91.48(2) 7_556 . ?
Sb9 Eu7 Sb6 172.40(3) 8 . ?
Sb6 Eu7 Sb6 81.21(4) 5_666 . ?
Sb5 Eu7 Eu5 55.139(19) 2_656 2_656 ?
Sb5 Eu7 Eu5 125.58(2) . 2_656 ?
Sb9 Eu7 Eu5 126.50(2) 7_556 2_656 ?
Sb9 Eu7 Eu5 57.319(18) 8 2_656 ?
Sb6 Eu7 Eu5 56.72(2) 5_666 2_656 ?
Sb6 Eu7 Eu5 119.11(3) . 2_656 ?
Sb5 Eu7 Eu5 125.58(2) 2_656 . ?
Sb5 Eu7 Eu5 55.139(19) . . ?
Sb9 Eu7 Eu5 57.319(18) 7_556 . ?
Sb9 Eu7 Eu5 126.50(2) 8 . ?
Sb6 Eu7 Eu5 119.11(3) 5_666 . ?
Sb6 Eu7 Eu5 56.72(2) . . ?
Eu5 Eu7 Eu5 175.30(3) 2_656 . ?
Sb5 Eu7 Eu3 57.73(2) 2_656 . ?
Sb5 Eu7 Eu3 123.64(2) . . ?
Sb9 Eu7 Eu3 53.531(18) 7_556 . ?
Sb9 Eu7 Eu3 134.60(3) 8 . ?
Sb6 Eu7 Eu3 119.40(3) 5_666 . ?
Sb6 Eu7 Eu3 52.19(2) . . ?
Eu5 Eu7 Eu3 110.763(14) 2_656 . ?
Eu5 Eu7 Eu3 68.832(14) . . ?
Sb5 Eu7 Eu3 123.64(2) 2_656 2_656 ?
Sb5 Eu7 Eu3 57.73(2) . 2_656 ?
Sb9 Eu7 Eu3 134.60(3) 7_556 2_656 ?
Sb9 Eu7 Eu3 53.531(18) 8 2_656 ?
Sb6 Eu7 Eu3 52.19(2) 5_666 2_656 ?
Sb6 Eu7 Eu3 119.40(3) . 2_656 ?
Eu5 Eu7 Eu3 68.832(14) 2_656 2_656 ?
Eu5 Eu7 Eu3 110.763(14) . 2_656 ?
Eu3 Eu7 Eu3 170.77(3) . 2_656 ?
Mn2 Sb1 Eu4 69.52(5) 1_556 6_566 ?
Mn2 Sb1 Eu4 69.52(5) 1_556 1_556 ?
Eu4 Sb1 Eu4 86.78(4) 6_566 1_556 ?
Mn2 Sb1 Eu5 133.810(19) 1_556 6_565 ?
Eu4 Sb1 Eu5 77.46(2) 6_566 6_565 ?
Eu4 Sb1 Eu5 140.49(4) 1_556 6_565 ?
Mn2 Sb1 Eu5 133.810(19) 1_556 . ?
Eu4 Sb1 Eu5 140.49(4) 6_566 . ?
Eu4 Sb1 Eu5 77.46(2) 1_556 . ?
Eu5 Sb1 Eu5 92.03(4) 6_565 . ?
Mn2 Sb1 Eu1 77.29(5) 1_556 . ?
Eu4 Sb1 Eu1 146.59(4) 6_566 . ?
Eu4 Sb1 Eu1 85.196(19) 1_556 . ?
Eu5 Sb1 Eu1 126.47(4) 6_565 . ?
Eu5 Sb1 Eu1 68.427(19) . . ?
Mn2 Sb1 Eu1 77.29(5) 1_556 5_566 ?
Eu4 Sb1 Eu1 85.196(19) 6_566 5_566 ?
Eu4 Sb1 Eu1 146.59(4) 1_556 5_566 ?
Eu5 Sb1 Eu1 68.427(19) 6_565 5_566 ?
Eu5 Sb1 Eu1 126.47(4) . 5_566 ?
Eu1 Sb1 Eu1 83.91(4) . 5_566 ?
Mn3 Sb2 Mn4 66.60(6) 2_556 . ?
Mn3 Sb2 Mn1 158.57(9) 2_556 . ?
Mn4 Sb2 Mn1 106.78(7) . . ?
Mn3 Sb2 Mn2 105.68(8) 2_556 5_565 ?
Mn4 Sb2 Mn2 156.50(9) . 5_565 ?
Mn1 Sb2 Mn2 71.93(7) . 5_565 ?
Mn3 Sb2 Eu2 79.33(5) 2_556 . ?
Mn4 Sb2 Eu2 79.31(5) . . ?
Mn1 Sb2 Eu2 79.39(7) . . ?
Mn2 Sb2 Eu2 77.40(7) 5_565 . ?
Mn3 Sb2 Eu1 79.08(5) 2_556 . ?
Mn4 Sb2 Eu1 117.44(5) . . ?
Mn1 Sb2 Eu1 120.51(7) . . ?
Mn2 Sb2 Eu1 80.79(7) 5_565 . ?
Eu2 Sb2 Eu1 143.68(3) . . ?
Mn3 Sb2 Eu5 114.89(5) 2_556 . ?
Mn4 Sb2 Eu5 76.96(5) . . ?
Mn1 Sb2 Eu5 81.60(7) . . ?
Mn2 Sb2 Eu5 124.90(7) 5_565 . ?
Eu2 Sb2 Eu5 143.67(3) . . ?
Eu1 Sb2 Eu5 72.45(2) . . ?
Mn1 Sb3 Mn2 143.91(10) . . ?
Mn1 Sb3 Eu2 77.22(5) . . ?
Mn2 Sb3 Eu2 75.50(5) . . ?
Mn1 Sb3 Eu2 77.22(5) . 5_565 ?
Mn2 Sb3 Eu2 75.50(5) . 5_565 ?
Eu2 Sb3 Eu2 80.83(4) . 5_565 ?
Mn1 Sb3 Eu3 67.27(5) . 6_565 ?
Mn2 Sb3 Eu3 133.74(3) . 6_565 ?
Eu2 Sb3 Eu3 144.26(4) . 6_565 ?
Eu2 Sb3 Eu3 87.43(2) 5_565 6_565 ?
Mn1 Sb3 Eu3 67.27(5) . . ?
Mn2 Sb3 Eu3 133.74(3) . . ?
Eu2 Sb3 Eu3 87.43(2) . . ?
Eu2 Sb3 Eu3 144.26(4) 5_565 . ?
Eu3 Sb3 Eu3 82.69(4) 6_565 . ?
Mn1 Sb3 Eu4 133.98(4) . 6_565 ?
Mn2 Sb3 Eu4 67.19(5) . 6_565 ?
Eu2 Sb3 Eu4 142.54(4) . 6_565 ?
Eu2 Sb3 Eu4 86.70(2) 5_565 6_565 ?
Eu3 Sb3 Eu4 69.21(2) 6_565 6_565 ?
Eu3 Sb3 Eu4 120.83(4) . 6_565 ?
Mn1 Sb3 Eu4 133.98(4) . . ?
Mn2 Sb3 Eu4 67.19(5) . . ?
Eu2 Sb3 Eu4 86.70(2) . . ?
Eu2 Sb3 Eu4 142.54(4) 5_565 . ?
Eu3 Sb3 Eu4 120.83(4) 6_565 . ?
Eu3 Sb3 Eu4 69.21(2) . . ?
Eu4 Sb3 Eu4 82.09(3) 6_565 . ?
Mn4 Sb4 Mn3 145.54(7) . 1_554 ?
Mn4 Sb4 Sb4 107.29(7) . 7 ?
Mn3 Sb4 Sb4 107.15(6) 1_554 7 ?
Mn4 Sb4 Eu6 78.86(5) . 7 ?
Mn3 Sb4 Eu6 79.34(5) 1_554 7 ?
Sb4 Sb4 Eu6 127.59(5) 7 7 ?
Mn4 Sb4 Eu2 76.66(5) . . ?
Mn3 Sb4 Eu2 76.44(5) 1_554 . ?
Sb4 Sb4 Eu2 143.84(5) 7 . ?
Eu6 Sb4 Eu2 88.57(3) 7 . ?
Mn4 Sb4 Eu4 130.96(5) . . ?
Mn3 Sb4 Eu4 66.81(5) 1_554 . ?
Sb4 Sb4 Eu4 65.41(3) 7 . ?
Eu6 Sb4 Eu4 146.13(3) 7 . ?
Eu2 Sb4 Eu4 84.64(2) . . ?
Mn4 Sb4 Eu4 66.03(5) . 7 ?
Mn3 Sb4 Eu4 129.74(5) 1_554 7 ?
Sb4 Sb4 Eu4 65.21(3) 7 7 ?
Eu6 Sb4 Eu4 71.36(2) 7 7 ?
Eu2 Sb4 Eu4 140.11(3) . 7 ?
Eu4 Sb4 Eu4 130.62(3) . 7 ?
Mn4 Sb4 Eu3 66.32(5) . . ?
Mn3 Sb4 Eu3 131.37(5) 1_554 . ?
Sb4 Sb4 Eu3 65.74(4) 7 . ?
Eu6 Sb4 Eu3 145.16(3) 7 . ?
Eu2 Sb4 Eu3 84.68(2) . . ?
Eu4 Sb4 Eu3 67.12(2) . . ?
Eu4 Sb4 Eu3 92.60(3) 7 . ?
Mn4 Sb4 Eu3 130.24(5) . 7 ?
Mn3 Sb4 Eu3 65.47(5) 1_554 7 ?
Sb4 Sb4 Eu3 65.36(3) 7 7 ?
Eu6 Sb4 Eu3 71.70(2) 7 7 ?
Eu2 Sb4 Eu3 139.44(3) . 7 ?
Eu4 Sb4 Eu3 92.51(3) . 7 ?
Eu4 Sb4 Eu3 66.94(2) 7 7 ?
Eu3 Sb4 Eu3 131.10(3) . 7 ?
Mn4 Sb5 Mn3 69.16(7) 7_556 8 ?
Mn4 Sb5 Sb7 141.45(6) 7_556 . ?
Mn3 Sb5 Sb7 143.31(6) 8 . ?
Mn4 Sb5 Eu6 80.24(5) 7_556 1_556 ?
Mn3 Sb5 Eu6 80.84(5) 8 1_556 ?
Sb7 Sb5 Eu6 85.67(4) . 1_556 ?
Mn4 Sb5 Eu7 126.24(6) 7_556 . ?
Mn3 Sb5 Eu7 86.18(5) 8 . ?
Sb7 Sb5 Eu7 84.75(3) . . ?
Eu6 Sb5 Eu7 143.50(3) 1_556 . ?
Mn4 Sb5 Eu5 88.21(6) 7_556 . ?
Mn3 Sb5 Eu5 128.01(6) 8 . ?
Sb7 Sb5 Eu5 81.42(3) . . ?
Eu6 Sb5 Eu5 142.35(3) 1_556 . ?
Eu7 Sb5 Eu5 70.21(2) . . ?
Mn4 Sb5 Eu3 128.56(6) 7_556 2_656 ?
Mn3 Sb5 Eu3 65.18(5) 8 2_656 ?
Sb7 Sb5 Eu3 78.16(3) . 2_656 ?
Eu6 Sb5 Eu3 70.49(2) 1_556 2_656 ?
Eu7 Sb5 Eu3 73.09(2) . 2_656 ?
Eu5 Sb5 Eu3 139.24(3) . 2_656 ?
Mn4 Sb5 Eu4 64.31(5) 7_556 1_556 ?
Mn3 Sb5 Eu4 127.58(5) 8 1_556 ?
Sb7 Sb5 Eu4 77.15(3) . 1_556 ?
Eu6 Sb5 Eu4 69.01(2) 1_556 1_556 ?
Eu7 Sb5 Eu4 141.52(3) . 1_556 ?
Eu5 Sb5 Eu4 73.66(2) . 1_556 ?
Eu3 Sb5 Eu4 133.60(3) 2_656 1_556 ?
Mn1 Sb6 Eu3 67.92(5) . . ?
Mn1 Sb6 Eu3 67.92(5) . 6_565 ?
Eu3 Sb6 Eu3 84.47(4) . 6_565 ?
Mn1 Sb6 Eu5 77.30(5) . 6_565 ?
Eu3 Sb6 Eu5 145.21(4) . 6_565 ?
Eu3 Sb6 Eu5 81.996(19) 6_565 6_565 ?
Mn1 Sb6 Eu5 77.30(5) . . ?
Eu3 Sb6 Eu5 81.996(19) . . ?
Eu3 Sb6 Eu5 145.21(4) 6_565 . ?
Eu5 Sb6 Eu5 91.20(4) 6_565 . ?
Mn1 Sb6 Eu7 130.61(2) . 5_666 ?
Eu3 Sb6 Eu7 138.93(4) . 5_666 ?
Eu3 Sb6 Eu7 74.528(18) 6_565 5_666 ?
Eu5 Sb6 Eu7 66.537(17) 6_565 5_666 ?
Eu5 Sb6 Eu7 133.37(4) . 5_666 ?
Mn1 Sb6 Eu7 130.61(2) . . ?
Eu3 Sb6 Eu7 74.528(18) . . ?
Eu3 Sb6 Eu7 138.93(4) 6_565 . ?
Eu5 Sb6 Eu7 133.37(4) 6_565 . ?
Eu5 Sb6 Eu7 66.537(17) . . ?
Eu7 Sb6 Eu7 98.79(4) 5_666 . ?
Sb5 Sb7 Sb5 175.91(6) 6_565 . ?
Sb8 Sb8 Eu6 61.92(2) 5_665 5_665 ?
Sb8 Sb8 Eu6 61.92(2) 5_665 . ?
Eu6 Sb8 Eu6 123.84(4) 5_665 . ?
Sb8 Sb8 Eu4 121.09(4) 5_665 . ?
Eu6 Sb8 Eu4 144.49(4) 5_665 . ?
Eu6 Sb8 Eu4 70.859(17) . . ?
Sb8 Sb8 Eu4 121.09(4) 5_665 6_565 ?
Eu6 Sb8 Eu4 70.860(17) 5_665 6_565 ?
Eu6 Sb8 Eu4 144.49(4) . 6_565 ?
Eu4 Sb8 Eu4 80.64(4) . 6_565 ?
Sb8 Sb8 Eu3 121.92(5) 5_665 6_565 ?
Eu6 Sb8 Eu3 71.359(16) 5_665 6_565 ?
Eu6 Sb8 Eu3 144.82(4) . 6_565 ?
Eu4 Sb8 Eu3 116.99(4) . 6_565 ?
Eu4 Sb8 Eu3 67.67(2) 6_565 6_565 ?
Sb8 Sb8 Eu3 121.92(5) 5_665 . ?
Eu6 Sb8 Eu3 144.82(4) 5_665 . ?
Eu6 Sb8 Eu3 71.359(16) . . ?
Eu4 Sb8 Eu3 67.67(2) . . ?
Eu4 Sb8 Eu3 116.99(4) 6_565 . ?
Eu3 Sb8 Eu3 80.23(3) 6_565 . ?
Mn3 Sb9 Mn4 111.85(7) . 7_556 ?
Mn3 Sb9 Eu7 82.98(5) . 7_556 ?
Mn4 Sb9 Eu7 129.48(5) 7_556 7_556 ?
Mn3 Sb9 Eu5 130.74(5) . . ?
Mn4 Sb9 Eu5 84.24(5) 7_556 . ?
Eu7 Sb9 Eu5 123.18(3) 7_556 . ?
Mn3 Sb9 Eu4 68.84(5) . 1_556 ?
Mn4 Sb9 Eu4 68.01(5) 7_556 1_556 ?
Eu7 Sb9 Eu4 151.57(3) 7_556 1_556 ?
Eu5 Sb9 Eu4 76.11(2) . 1_556 ?
Mn3 Sb9 Eu5 141.78(5) . 7_556 ?
Mn4 Sb9 Eu5 73.76(5) 7_556 7_556 ?
Eu7 Sb9 Eu5 67.41(2) 7_556 7_556 ?
Eu5 Sb9 Eu5 86.80(2) . 7_556 ?
Eu4 Sb9 Eu5 139.27(3) 1_556 7_556 ?
Mn3 Sb9 Eu3 67.67(5) . 7_556 ?
Mn4 Sb9 Eu3 68.25(5) 7_556 7_556 ?
Eu7 Sb9 Eu3 74.85(2) 7_556 7_556 ?
Eu5 Sb9 Eu3 152.08(3) . 7_556 ?
Eu4 Sb9 Eu3 96.94(3) 1_556 7_556 ?
Eu5 Sb9 Eu3 81.18(2) 7_556 7_556 ?
Mn3 Sb9 Eu1 74.32(5) . . ?
Mn4 Sb9 Eu1 143.12(5) 7_556 . ?
Eu7 Sb9 Eu1 86.82(3) 7_556 . ?
Eu5 Sb9 Eu1 67.41(2) . . ?
Eu4 Sb9 Eu1 82.14(2) 1_556 . ?
Eu5 Sb9 Eu1 124.94(3) 7_556 . ?
Eu3 Sb9 Eu1 139.29(3) 7_556 . ?
Sb2 Mn1 Sb2 104.32(10) . 6_565 ?
Sb2 Mn1 Sb3 110.20(8) . . ?
Sb2 Mn1 Sb3 110.20(8) 6_565 . ?
Sb2 Mn1 Sb6 111.25(8) . . ?
Sb2 Mn1 Sb6 111.25(8) 6_565 . ?
Sb3 Mn1 Sb6 109.53(10) . . ?
Sb2 Mn1 Eu3 168.18(8) . 6_565 ?
Sb2 Mn1 Eu3 87.50(3) 6_565 6_565 ?
Sb3 Mn1 Eu3 64.66(5) . 6_565 ?
Sb6 Mn1 Eu3 63.17(5) . 6_565 ?
Sb2 Mn1 Eu3 87.50(3) . . ?
Sb2 Mn1 Eu3 168.18(8) 6_565 . ?
Sb3 Mn1 Eu3 64.66(5) . . ?
Sb6 Mn1 Eu3 63.17(5) . . ?
Eu3 Mn1 Eu3 80.68(6) 6_565 . ?
Sb2 Mn1 Eu2 55.40(5) . . ?
Sb2 Mn1 Eu2 108.13(9) 6_565 . ?
Sb3 Mn1 Eu2 56.85(5) . . ?
Sb6 Mn1 Eu2 140.56(5) . . ?
Eu3 Mn1 Eu2 121.38(8) 6_565 . ?
Eu3 Mn1 Eu2 78.47(4) . . ?
Sb2 Mn1 Eu2 108.13(9) . 5_565 ?
Sb2 Mn1 Eu2 55.40(5) 6_565 5_565 ?
Sb3 Mn1 Eu2 56.85(5) . 5_565 ?
Sb6 Mn1 Eu2 140.56(5) . 5_565 ?
Eu3 Mn1 Eu2 78.47(4) 6_565 5_565 ?
Eu3 Mn1 Eu2 121.38(8) . 5_565 ?
Eu2 Mn1 Eu2 67.64(6) . 5_565 ?
Sb2 Mn2 Sb2 103.37(10) 5_565 2 ?
Sb2 Mn2 Sb1 110.84(8) 5_565 1_554 ?
Sb2 Mn2 Sb1 110.84(8) 2 1_554 ?
Sb2 Mn2 Sb3 112.12(8) 5_565 . ?
Sb2 Mn2 Sb3 112.12(8) 2 . ?
Sb1 Mn2 Sb3 107.59(11) 1_554 . ?
Sb2 Mn2 Eu4 88.13(3) 5_565 6_565 ?
Sb2 Mn2 Eu4 168.19(8) 2 6_565 ?
Sb1 Mn2 Eu4 61.52(5) 1_554 6_565 ?
Sb3 Mn2 Eu4 64.81(6) . 6_565 ?
Sb2 Mn2 Eu4 168.19(8) 5_565 . ?
Sb2 Mn2 Eu4 88.13(3) 2 . ?
Sb1 Mn2 Eu4 61.52(5) 1_554 . ?
Sb3 Mn2 Eu4 64.81(6) . . ?
Eu4 Mn2 Eu4 80.27(7) 6_565 . ?
Sb2 Mn2 Eu2 56.35(4) 5_565 5_565 ?
Sb2 Mn2 Eu2 109.60(9) 2 5_565 ?
Sb1 Mn2 Eu2 139.48(6) 1_554 5_565 ?
Sb3 Mn2 Eu2 57.84(5) . 5_565 ?
Eu4 Mn2 Eu2 78.89(4) 6_565 5_565 ?
Eu4 Mn2 Eu2 122.56(9) . 5_565 ?
Sb2 Mn2 Eu2 109.60(9) 5_565 . ?
Sb2 Mn2 Eu2 56.35(4) 2 . ?
Sb1 Mn2 Eu2 139.48(6) 1_554 . ?
Sb3 Mn2 Eu2 57.84(5) . . ?
Eu4 Mn2 Eu2 122.56(9) 6_565 . ?
Eu4 Mn2 Eu2 78.89(4) . . ?
Eu2 Mn2 Eu2 69.07(6) 5_565 . ?
Sb5 Mn3 Sb2 107.47(8) 8_455 2_556 ?
Sb5 Mn3 Sb9 105.12(8) 8_455 . ?
Sb2 Mn3 Sb9 115.91(8) 2_556 . ?
Sb5 Mn3 Sb4 108.43(8) 8_455 1_556 ?
Sb2 Mn3 Sb4 112.64(8) 2_556 1_556 ?
Sb9 Mn3 Sb4 106.82(8) . 1_556 ?
Sb5 Mn3 Mn4 55.40(6) 8_455 2_556 ?
Sb2 Mn3 Mn4 56.85(6) 2_556 2_556 ?
Sb9 Mn3 Mn4 145.31(10) . 2_556 ?
Sb4 Mn3 Mn4 106.77(8) 1_556 2_556 ?
Sb5 Mn3 Eu3 70.85(5) 8_455 7_556 ?
Sb2 Mn3 Eu3 178.28(8) 2_556 7_556 ?
Sb9 Mn3 Eu3 65.18(5) . 7_556 ?
Sb4 Mn3 Eu3 67.89(5) 1_556 7_556 ?
Mn4 Mn3 Eu3 121.47(8) 2_556 7_556 ?
Sb5 Mn3 Eu4 164.03(8) 8_455 1_556 ?
Sb2 Mn3 Eu4 88.24(6) 2_556 1_556 ?
Sb9 Mn3 Eu4 64.06(5) . 1_556 ?
Sb4 Mn3 Eu4 66.48(5) 1_556 1_556 ?
Mn4 Mn3 Eu4 140.02(8) 2_556 1_556 ?
Eu3 Mn3 Eu4 93.46(5) 7_556 1_556 ?
Sb5 Mn3 Eu6 55.53(4) 8_455 7_556 ?
Sb2 Mn3 Eu6 113.54(7) 2_556 7_556 ?
Sb9 Mn3 Eu6 130.43(7) . 7_556 ?
Sb4 Mn3 Eu6 54.80(4) 1_556 7_556 ?
Mn4 Mn3 Eu6 66.15(6) 2_556 7_556 ?
Eu3 Mn3 Eu6 65.30(4) 7_556 7_556 ?
Eu4 Mn3 Eu6 121.27(6) 1_556 7_556 ?
Sb5 Mn3 Eu2 113.11(7) 8_455 1_556 ?
Sb2 Mn3 Eu2 55.58(4) 2_556 1_556 ?
Sb9 Mn3 Eu2 141.63(7) . 1_556 ?
Sb4 Mn3 Eu2 58.37(4) 1_556 1_556 ?
Mn4 Mn3 Eu2 66.75(6) 2_556 1_556 ?
Eu3 Mn3 Eu2 124.55(6) 7_556 1_556 ?
Eu4 Mn3 Eu2 77.86(4) 1_556 1_556 ?
Eu6 Mn3 Eu2 73.21(4) 7_556 1_556 ?
Sb5 Mn3 Eu1 110.18(7) 8_455 . ?
Sb2 Mn3 Eu1 55.90(4) 2_556 . ?
Sb9 Mn3 Eu1 61.52(4) . . ?
Sb4 Mn3 Eu1 141.36(7) 1_556 . ?
Mn4 Mn3 Eu1 96.07(7) 2_556 . ?
Eu3 Mn3 Eu1 124.80(6) 7_556 . ?
Eu4 Mn3 Eu1 75.93(4) 1_556 . ?
Eu6 Mn3 Eu1 161.26(6) 7_556 . ?
Eu2 Mn3 Eu1 106.16(5) 1_556 . ?
Sb5 Mn4 Sb2 107.23(8) 7_556 . ?
Sb5 Mn4 Sb9 103.99(8) 7_556 7_556 ?
Sb2 Mn4 Sb9 116.59(8) . 7_556 ?
Sb5 Mn4 Sb4 109.38(8) 7_556 . ?
Sb2 Mn4 Sb4 112.33(8) . . ?
Sb9 Mn4 Sb4 106.86(7) 7_556 . ?
Sb5 Mn4 Mn3 55.44(6) 7_556 2_556 ?
Sb2 Mn4 Mn3 56.56(6) . 2_556 ?
Sb9 Mn4 Mn3 144.54(9) 7_556 2_556 ?
Sb4 Mn4 Mn3 107.38(9) . 2_556 ?
Sb5 Mn4 Eu4 72.10(5) 7_556 7 ?
Sb2 Mn4 Eu4 178.86(9) . 7 ?
Sb9 Mn4 Eu4 64.53(5) 7_556 7 ?
Sb4 Mn4 Eu4 67.21(5) . 7 ?
Mn3 Mn4 Eu4 122.46(8) 2_556 7 ?
Sb5 Mn4 Eu3 165.03(8) 7_556 . ?
Sb2 Mn4 Eu3 87.16(6) . . ?
Sb9 Mn4 Eu3 64.71(5) 7_556 . ?
Sb4 Mn4 Eu3 67.29(5) . . ?
Mn3 Mn4 Eu3 139.37(8) 2_556 . ?
Eu4 Mn4 Eu3 93.57(5) 7 . ?
Sb5 Mn4 Eu5 108.51(7) 7_556 . ?
Sb2 Mn4 Eu5 57.17(4) . . ?
Sb9 Mn4 Eu5 61.05(5) 7_556 . ?
Sb4 Mn4 Eu5 142.04(7) . . ?
Mn3 Mn4 Eu5 95.83(7) 2_556 . ?
Eu4 Mn4 Eu5 123.87(6) 7 . ?
Eu3 Mn4 Eu5 75.48(4) . . ?
Sb5 Mn4 Eu6 55.91(4) 7_556 7 ?
Sb2 Mn4 Eu6 114.00(7) . 7 ?
Sb9 Mn4 Eu6 129.24(7) 7_556 7 ?
Sb4 Mn4 Eu6 55.18(4) . 7 ?
Mn3 Mn4 Eu6 66.97(6) 2_556 7 ?
Eu4 Mn4 Eu6 64.86(4) 7 7 ?
Eu3 Mn4 Eu6 122.47(6) . 7 ?
Eu5 Mn4 Eu6 161.13(6) . 7 ?
Sb5 Mn4 Eu2 113.00(7) 7_556 . ?
Sb2 Mn4 Eu2 55.47(4) . . ?
Sb9 Mn4 Eu2 142.87(7) 7_556 . ?
Sb4 Mn4 Eu2 58.34(4) . . ?
Mn3 Mn4 Eu2 66.59(6) 2_556 . ?
Eu4 Mn4 Eu2 123.82(6) 7 . ?
Eu3 Mn4 Eu2 78.31(4) . . ?
Eu5 Mn4 Eu2 107.79(5) . . ?
Eu6 Mn4 Eu2 73.43(4) 7 . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Eu1 Sb2 3.2367(9) . ?
Eu1 Sb2 3.2367(9) 2_556 ?
Eu1 Sb1 3.4087(11) . ?
Eu1 Sb1 3.4087(11) 5_566 ?
Eu1 Sb9 3.5038(11) 2_556 ?
Eu1 Sb9 3.5038(10) . ?
Eu1 Eu5 3.8321(6) . ?
Eu1 Eu5 3.8321(6) 2_556 ?
Eu1 Mn3 3.838(2) 2_556 ?
Eu1 Mn3 3.838(2) . ?
Eu2 Sb2 3.2203(9) 2 ?
Eu2 Sb2 3.2203(9) . ?
Eu2 Sb3 3.3013(11) . ?
Eu2 Sb3 3.3013(11) 5_565 ?
Eu2 Sb4 3.3602(11) 2 ?
Eu2 Sb4 3.3602(11) . ?
Eu2 Mn2 3.775(3) 5_565 ?
Eu2 Mn2 3.775(3) . ?
Eu2 Mn3 3.837(2) 1_554 ?
Eu2 Mn3 3.837(2) 2_556 ?
Eu2 Mn4 3.841(2) 2 ?
Eu2 Mn4 3.841(2) . ?
Eu3 Sb6 3.3819(12) . ?
Eu3 Sb9 3.4374(11) 7_556 ?
Eu3 Sb3 3.4414(12) . ?
Eu3 Mn3 3.503(2) 7_556 ?
Eu3 Mn1 3.512(2) . ?
Eu3 Sb8 3.5282(12) . ?
Eu3 Mn4 3.531(2) . ?
Eu3 Sb4 3.5568(12) . ?
Eu3 Sb4 3.5677(11) 7 ?
Eu3 Sb5 3.6462(12) 2_656 ?
Eu3 Eu4 3.9155(10) . ?
Eu3 Eu6 3.9684(7) . ?
Eu4 Sb1 3.3008(12) 1_554 ?
Eu4 Sb9 3.4088(11) 1_554 ?
Eu4 Sb3 3.4532(11) . ?
Eu4 Mn4 3.501(2) 7 ?
Eu4 Sb8 3.5042(12) . ?
Eu4 Mn2 3.518(2) . ?
Eu4 Sb4 3.5264(11) . ?
Eu4 Sb4 3.5322(12) 7 ?
Eu4 Mn3 3.535(2) 1_554 ?
Eu4 Sb5 3.6970(11) 1_554 ?
Eu4 Eu6 3.9295(8) . ?
Eu5 Sb2 3.2476(12) . ?
Eu5 Sb5 3.2829(12) . ?
Eu5 Sb9 3.4002(10) . ?
Eu5 Sb1 3.4066(10) . ?
Eu5 Sb6 3.4308(11) . ?
Eu5 Sb9 3.4318(10) 7_556 ?
Eu5 Eu7 3.7645(6) . ?
Eu5 Mn4 3.765(2) . ?
Eu5 Eu4 4.1973(9) 1_556 ?
Eu6 Sb4 3.1882(12) 7 ?
Eu6 Sb4 3.1882(12) 8 ?
Eu6 Sb5 3.2019(9) 1_554 ?
Eu6 Sb5 3.2019(9) 2_656 ?
Eu6 Sb8 3.2659(11) 5_665 ?
Eu6 Sb8 3.2659(11) . ?
Eu6 Mn4 3.810(2) 7 ?
Eu6 Mn4 3.810(2) 8 ?
Eu6 Mn3 3.834(2) 8_554 ?
Eu6 Mn3 3.834(2) 7_556 ?
Eu6 Eu4 3.9295(8) 2_655 ?
Eu7 Sb5 3.2634(9) 2_656 ?
Eu7 Sb5 3.2634(9) . ?
Eu7 Sb9 3.3508(11) 7_556 ?
Eu7 Sb9 3.3508(11) 8 ?
Eu7 Sb6 3.4318(11) 5_666 ?
Eu7 Sb6 3.4318(11) . ?
Eu7 Eu5 3.7645(6) 2_656 ?
Eu7 Eu3 4.1258(8) 2_656 ?
Sb1 Mn2 2.832(3) 1_556 ?
Sb1 Eu4 3.3008(12) 6_566 ?
Sb1 Eu4 3.3008(12) 1_556 ?
Sb1 Eu5 3.4066(10) 6_565 ?
Sb1 Eu1 3.4087(11) 5_566 ?
Sb2 Mn3 2.765(2) 2_556 ?
Sb2 Mn4 2.774(2) . ?
Sb2 Mn1 2.776(2) . ?
Sb2 Mn2 2.794(2) 5_565 ?
Sb3 Mn1 2.833(3) . ?
Sb3 Mn2 2.836(3) . ?
Sb3 Eu2 3.3013(11) 5_565 ?
Sb3 Eu3 3.4414(12) 6_565 ?
Sb3 Eu4 3.4532(11) 6_565 ?
Sb4 Mn4 2.792(2) . ?
Sb4 Mn3 2.800(2) 1_554 ?
Sb4 Sb4 2.9486(19) 7 ?
Sb4 Eu6 3.1882(12) 7 ?
Sb4 Eu4 3.5322(12) 7 ?
Sb4 Eu3 3.5677(11) 7 ?
Sb5 Mn4 2.679(2) 7_556 ?
Sb5 Mn3 2.680(2) 8 ?
Sb5 Sb7 3.0151(10) . ?
Sb5 Eu6 3.2019(9) 1_556 ?
Sb5 Eu3 3.6462(12) 2_656 ?
Sb5 Eu4 3.6970(11) 1_556 ?
Sb6 Mn1 2.856(3) . ?
Sb6 Eu3 3.3819(12) 6_565 ?
Sb6 Eu5 3.4308(11) 6_565 ?
Sb6 Eu7 3.4318(11) 5_666 ?
Sb7 Sb5 3.0151(10) 6_565 ?
Sb8 Sb8 3.074(3) 5_665 ?
Sb8 Eu6 3.2659(11) 5_665 ?
Sb8 Eu4 3.5042(12) 6_565 ?
Sb8 Eu3 3.5282(12) 6_565 ?
Sb9 Mn3 2.777(2) . ?
Sb9 Mn4 2.782(2) 7_556 ?
Sb9 Eu7 3.3508(11) 7_556 ?
Sb9 Eu4 3.4088(11) 1_556 ?
Sb9 Eu5 3.4318(10) 7_556 ?
Sb9 Eu3 3.4374(11) 7_556 ?
Mn1 Sb2 2.776(2) 6_565 ?
Mn1 Eu3 3.512(2) 6_565 ?
Mn1 Eu2 3.845(3) 5_565 ?
Mn2 Sb2 2.794(2) 5_565 ?
Mn2 Sb2 2.794(2) 2 ?
Mn2 Sb1 2.832(3) 1_554 ?
Mn2 Eu4 3.518(2) 6_565 ?
Mn2 Eu2 3.775(3) 5_565 ?
Mn3 Sb5 2.680(2) 8_455 ?
Mn3 Sb2 2.765(2) 2_556 ?
Mn3 Sb4 2.800(2) 1_556 ?
Mn3 Mn4 3.041(3) 2_556 ?
Mn3 Eu3 3.503(2) 7_556 ?
Mn3 Eu4 3.535(2) 1_556 ?
Mn3 Eu6 3.834(2) 7_556 ?
Mn3 Eu2 3.837(2) 1_556 ?
Mn4 Sb5 2.679(2) 7_556 ?
Mn4 Sb9 2.782(2) 7_556 ?
Mn4 Mn3 3.041(3) 2_556 ?
Mn4 Eu4 3.501(2) 7 ?
Mn4 Eu6 3.810(2) 7 ?
